Home >
Documents >
A stability-reversibility map unifies elasticity ... · A stability-reversibility map unifies...

Share this document with a friend

13

Transcript

SC I ENCE ADVANCES | R E S EARCH ART I C L E

PHYS I CS

1Cybermedia Center, Osaka University, Toyonaka, Osaka 560-0043, Japan. 2CASKey Laboratory of Theoretical Physics, Institute of Theoretical Physics, ChineseAcademy of Sciences, Beijing 100190, China. 3Institut de Physique Théorique, Uni-versité Paris Saclay, CNRS, CEA, F-91191 Gif-sur-Yvette, France. 4Laboratoire de Phy-sique Théorique, Département de physique de l’ENS, École Normale Supérieure, PSLResearch University, Sorbonne Universités, CNRS, 75005 Paris, France. 5GraduateSchool of Science, Osaka University, Toyonaka, Osaka 560-0043, Japan.*Corresponding author. Email: [email protected] (Y.J.); [email protected] (H.Y.)

Jin et al., Sci. Adv. 2018;4 : eaat6387 7 December 2018

Copyright © 2018

The Authors, some

rights reserved;

exclusive licensee

American Association

for the Advancement

of Science. No claim to

originalU.S. Government

Works. Distributed

under a Creative

Commons Attribution

NonCommercial

License 4.0 (CC BY-NC).

Dow

nloaded fro

A stability-reversibility map unifies elasticity, plasticity,yielding, and jamming in hard sphere glassesYuliang Jin1,2*, Pierfrancesco Urbani3, Francesco Zamponi4, Hajime Yoshino1,5*

Amorphous solids, such as glasses, have complex responses to deformations, with substantial consequences inmaterial design and applications. In this respect, two intertwined aspects are important: stability and reversibility. Itis crucial to understand, on the one hand, how a glass may become unstable due to increased plasticity under sheardeformations, and, on theother hand, towhat extent the response is reversible,meaning howmuch a system is able torecover the original configuration once the perturbation is released. Here, we focus on assemblies of hard spheres asthe simplest model of amorphous solids such as colloidal glasses and granular matter. We prepare glass statesquenched from equilibrium supercooled liquid states, which are obtained by using the swap Monte Carlo algorithmand correspond to a wide range of structural relaxation time scales. We exhaustively map out their stability and re-versibility under volume and shear strains using extensive numerical simulations. The region on the volume-shearstrain phase diagram where the original glass state remains solid is bounded by the shear yielding and the shearjamming lines that meet at a yielding-jamming crossover point. This solid phase can be further divided into two sub-phases: the stable glass phase, where the system deforms purely elastically and is totally reversible, and the marginalglass phase, where it experiences stochastic plastic deformations at mesoscopic scales and is partially irreversible. Thedetails of the stability-reversibilitymap depend strongly on the quality of annealing of the glass. This study provides aunified framework for understanding elasticity, plasticity, yielding, and jamming in amorphous solids.

hm

on March 29, 2020ttp://advances.sciencem

ag.org/

INTRODUCTIONUnderstanding the response of amorphousmaterials to deformations isa central problem in condensed matter both from fundamental andpractical viewpoints. It is not only a way to probe the nature of amor-phous solids and their properties but also crucial to understand a widerange of phenomena from the fracture ofmetallic glasses to earthquakesand landslides. Furthermore, it has important applications in materialdesign (1). Although many research efforts have focused on the mecha-nisms leading to the formation of amorphous solids from liquids (2–5),an orthogonal approach is to study these materials deep inside theiramorphous phase (6–8). In this work, we focus on this second strategyby addressing the problem of understanding the nature of the responseof glasses to volume and shear strains.

To a first approximation, glasses are solids much like crystals: Theydeform essentially elastically for small deformations but yield underlarge enough shear strains and start to flow.However, glasses are funda-mentally different from crystals, being out-of-equilibrium states ofmatter. As a consequence, the properties of glasses strongly dependon the details of the preparation protocol (3). As an example, the yieldingof glasses prepared via a fast quenchor very slowannealing is qualitativelydifferent (9). Thus, in sharp contrast to ordinary states of matter such asgases, liquids, and crystals, the equationsof state (EOS), or the constitutivelaws, of glasses, which characterize their macroscopic properties, mustdepend on the preparation protocol.Understanding themechanical prop-erties of glasses fromaunifiedmicroscopic point of view thus emerges as achallenging problem (10).

To this aim, a central question is to understand the degree of stabilityof a glass, i.e., to what extent it can resist deformations. In isotropicmaterials such as glasses, it is sufficient to consider two types of defor-mations, namely, the volume strain, which changes the volume of thesystem isotropically, and the shear strain, which preserves the volumebut changes the shape of the container. Under volume strains, glassesmelt by decompression, and in the presence of a hard-core repulsion, asin granularmatter and in colloids, they exhibit jamming upon compres-sion. The melting and the jamming transitions delimit the line wherethe glass remains solid. Taking a glass on that line, one can probe itsstability along the other axis of deformation, i.e., shear strain. Typically,the response of a glass to shear can be either (i) purely elastic and stable(note that this does not mean that the response is purely affine, as elas-ticity can emerge even in the presence of a nonaffine response), (ii) par-tially plastic (6–8), which is accompanied by slip avalanches and mightbe associated to the property of marginal stability (4, 11), or (iii) purelyplastic and unstable, once yielding takes place (7, 10, 12). Furthermore,granular materials (13) and dense suspensions (14) may (iv) jam whenthey are sheared.

A question related to stability is reversibility, i.e., to what extent aglass can recover its initial configuration when the deformation is re-leased. This question has been one of the key interests in cyclic shearexperiments of colloidal suspensions (15). In simulations of somemodelglasses, it has been found that a reversible-irreversible transition accom-panies the occurrence of yielding (16–18).

The purpose of this work was to study, through extensive numericalsimulations, the volume and shear strain phase diagramof amodel glassformer, hard spheres (HSs), to unify the abovementioned phenomena,i.e., plasticity, yielding, compression and shear jamming, and the failureof reversibility. Thanks to the swap algorithm, introducedbyKranendonkand Frenkel (19) and recently adapted to simulate polydisperse HS sys-tems with unprecedented efficiency (20), we are able to prepare initialequilibrium supercooled liquid configurations up to high densities goingeven beyond experimental limits (21). While the standard molecular dy-namics (MD) algorithm mimics the real dynamics, the swap algorithm

1 of 12

SC I ENCE ADVANCES | R E S EARCH ART I C L E

on March 29, 2020

http://advances.sciencemag.org/

Dow

nloaded from

accelerates the relaxation by introducing artificial exchanges of particlesat different positions. With this trick, a dense supercooled liquid statewith very large relaxation time can be prepared. Given such a system, byturning off the swapmoves and switching to standardMD simulations,the system is effectively confined in a glass state, because its relaxationtime is much larger than the achievable MD simulation time. By per-turbing this initial equilibrium state with a given rate of compression,decompression, or shear strain duringMD simulations, the system isdriven out of the original equilibrium supercooled liquid state. Inthis way, we study the out-of-equilibrium response to these externalperturbations of the glass selected by the initial supercooled liquidconfiguration, thus realizing what in (22) is called adiabatic statefollowing. Using this procedure, we completely map out the degreeof stability of the HS glasses corresponding to widely different prep-aration protocols. We show that there is a unique mapping betweendifferent types of stability and reversibility, that the stable and the mar-ginally stable glass phases can be well separated by sensitive measure-ment protocols (23, 24), and that marginality is manifested by a newtype of reversibility, which we denote as partial irreversibility.

The idea of establishing a phase diagram to unify the glass transition,jamming, and yielding of amorphous solids was initially proposed byLiu and Nagel (4, 25) and subsequently explored by others [e.g., see(26, 27)]. Here, we explicitly construct such a phase diagram for HSglasses, represented by a stability-reversibilitymap, which complementsthe conjecture in (4) with new ingredients, namely, the existence of themarginal glass phase and the dependence on the quality of annealing(22, 28, 29). Our phase diagram is expected to be reproducible inexperiments on vibrated granular glasses (30, 31) and colloids (10),while molecular glasses are usually described by soft potentials, forwhich the phase diagram needs to be modified.

The plasticity of amorphous solids has been extensively studied inboth phenomenological (12, 32–34) and first principle (5, 29) theories.According to the exact mean-field (MF) solution of the HS model ininfinite dimensions (29), the glass phase can be decomposed into stableregions where plasticity is absent, andmarginally stable regions where itis expected. The two phases are separated by a line where the so-calledGardner transition takes place (5, 23, 24). Determiningwhether thisMFGardner transition is also present in three dimensions is an extremelyhard and currently open problem. Numerical simulations in threedimensions have found consistent evidence that an HS glass changesfrom a stable state to a marginally stable state across a certain thresholddensity before reaching jamming (23, 24) but are not capable to deter-mine whether such a change corresponds to a phase transition or acrossover, because of the lack of a careful analysis of finite size effects.Here, we relate the signatures of the Gardner transition/crossover to theemergence of plastic behavior and avalanches (11, 35, 36), which can bemeasured in simulations via the onset of partial plasticity and the emer-gence of a protocol-dependent shear modulus (24, 37). The Gardnerthreshold determined in this approach is consistent with an independentestimate based on the growth of a spin glass–like susceptibility (23). Be-cause the scope of our work is not to decide on the existence of a sharpGardner phase transition, here we keep the conventional use of theterminology “Gardner transition” but do not exclude the possibilitythat it may become a crossover in three dimensions. Moreover, it re-mains an open question whether the Gardner transition and the as-sociated marginality are of relevance to other systems. For example,the absence of marginality has been reported in simulations of a three-dimensional soft potential model (38) and a system of HSs confinedin a one-dimensional channel (39).While details may change among

Jin et al., Sci. Adv. 2018;4 : eaat6387 7 December 2018

various systems, the approach used in this study provides an exampleof how to construct a stability-reversibility map for generic glasses.

RESULTSPreparation of annealed glassesWe study a three-dimensional HS glass with continuous polydispersity,identical to the one in (20) (see Materials and Methods). Note that forHSs, the temperature is irrelevant: It only fixes the overall kinetic energyof the system, which is related to the sphere velocities, and thus to theunit of time. In our simulations, we set kBT to unity. The relevant con-trol parameters in this study are the packing fraction φ and the shearstrain g. The reduced or dimensionless pressure p = P/(kBTr), with Pbeing the pressure and r the number density, can be determineduniquely from the EOS for the given φ and g. Because the jamminglimit is the point where the reduced pressure of HSs diverges, it cor-responds, for our system, to the infinite pressure limit for fixed tem-perature or the zero-temperature limit for fixed pressure.

One can considerHSs as the limit of soft repulsive particles when theinteraction energy scale divided by kBT goes to infinity: Then, the HSsystem formally corresponds to the zero-temperature limit of soft repul-sive particles in the unjammed phase where particles do not overlap.The jamming limit coincides in both systems, but the overjammedphase is inaccessible by definition for HSs. As a consequence, one ofthe axes (the temperature axis) in the Liu-Nagel phase diagram (4) willbe missing in our context. The HS phase diagram established hereshould correspond to the zero-temperature plane of the Liu-Nagelphase diagram without the overjammed part.

Our HSmodel is chosen in such a way that the particle swap moves(19) can be used in combinationwith standard event-drivenMDto fullyequilibrate the system up to very high densities, covering a very widerange of time scales for the standard MD without swap (20). Switchingoff the swap movements at volume fraction φg and leaving only MDacting on the particles, one gets effectively an HS amorphous solid,corresponding to the glass that would be formed during an annealingprocess that falls out of equilibrium at φg. Therefore, φg is the glasstransition density. Because the system is still in equilibrium at φg, itsreduced pressure pg follows the liquid EOS (L-EOS) pg = pliq(φg).

The possibility to explore a wide range of glass transition densities,thanks to the swap algorithm, is crucial to ourwork. In the following, wechoose to work on three different values of φg, representing ascendinglevels of annealing:

1) Weakly annealed case: φg = 0.609, corresponding to the pressurepg = 25.9. Berthier et al. (21) fitted the data of a-relaxation time ta as afunction of p in liquids using the standard Vogel-Fulcher-Tammann(VFT) form ta = t∞ exp[A/(pvft − p)], a generalized VFT form ta =t∞ exp[A/(pvft − p)2], and the facilitation model (FM) form ta = t∞exp[A(p − pfm)

2] [see (21) for details on the fitting]. We estimate thatthe a-relaxation time corresponding to pg = 25.9 is about ta/t0 ~ 5 × 10

4

for all these forms, where t0 ~ 104 is the a-relaxation time at the onsetdensity φ0 ≈ 0.56 of glassy dynamics. Both VFT and FM forms giveconsistent values of ta. The time scale ta/t0 ~ 5 × 104 corresponds toa typical time scale measured experimentally in colloidal glasses(ta/t0 ≲ 105 s and t0 ≈ 10−1 s).

2) Moderately annealed case: φg = 0.631 and pg = 30.9. At this den-sity, the standard VFT fitting gives an estimated time scale ta/t0 ~ 3 ×1010, the generalized VFT gives ta/t0 ~ 1010, and the FM fitting givesta/t0 ~ 109. These time scales are typically reachable in molecularglass-forming liquids (ta/t0 ≲ 1013 s and t0 ≈ 10−10 s).

2 of 12

SC I ENCE ADVANCES | R E S EARCH ART I C L E

on March 29, 2020

http://advances.sciencemag.org/

Dow

nloaded from

3) Deeply annealed case: φg = 0.655 and pg = 40.0. At this density,the relaxation time is enormously large, and both VFT and FM fittingsare unreliable. Fullerton and Berthier (40) measured the stability ratioS(the ratio between themelting time and the equilibrium relaxation timeat themelting temperature) of this system.According to the data in (40),the stability ratio at this density is around S e 103 � 105 (the value de-pends on the melting pressure), which is comparable to experimentalscales S e 102 � 105 of vapor-deposited ultrastable glasses (41).

While the time scales we can access correspond to different materials,as discussed above, it is important to stress that molecular glass-formingliquids and ultrastable glasses do not display a hard-core repulsion. Therepulsion between molecules in these systems is usually better describedby a Lennard-Jones–like soft potential. Therefore, some of the phenome-na that we will describe in the following, which are strongly related to thepresence of a hard-core potential, will be absent in these materials. Themost important example is jamming, which is, by definition, not presentin Lennard-Jones–like soft potentials. The nature of the Gardner transi-tion could also be markedly different in some soft materials (38), and theapplicability of someof our results on partial irreversibility should then bechecked. Yet, we believe that theHSmodel is a remarkable benchmark asit displays many important instability mechanisms (melting, yielding,compression and shear jamming, and the onset of marginal stability).It thus allows us to study in full detail the interplay between these in-stability mechanisms and their dependence on the quality of annealing.

Stability and reversibilityStarting from the equilibrated supercooled liquid configurations at φg,we now turn off the swap moves. By doing this, the liquid relaxationtime goes beyond the time scale that we can access in our numericalexperiments, and the system is thus effectively trapped into a glassstate.We can then follow the quasi-static evolution of the system un-der slow changes of the volume strain D = (φg − φ)/φ and the shearstrain g (seeMaterials andMethods) andmeasure the correspondingevolution of the pressure and the shear stress. Although the system isformally out of equilibrium (from the liquid point of view), one canreach a perfectly stationary state on the time scale we explore, restrictedto the glass basin (22). The basin can then be followed in restrictedmetastable “equilibrium.” We call the resulting trajectory in controlparameter space metastable EOS or glass EOS (G-EOS) to distinguishit from the L-EOS. The G-EOS can be obtained by plotting the pressureand stress as functions of the volume and shear strains.

The change of volume strain D can be converted to that of volumefraction φ via the relationφ = φg/(1 + D). To achieve a change in volumefraction, all particle diametersD are uniformly changedwith rate

:D=D ¼

2� 10�4 for compression and:D=D ¼ �2� 10�4 for decompression.

The resulting rate of the change of volume strain is:D ¼ �3ð1þ DÞ

:DD .

The change of the shear strain is given at a rate:g ¼ 10�4. The cor-

responding time scales of these rates are in between the fast b- andthe a-relaxation times, in such a way that the glass is followed nearlyadiabatically, while the a-relaxation remains effectively frozen (23, 24).The target strains (D, g) can be achieved starting from the initial point(0, 0) following various paths in the volume-shear strain plane. Forexample, one can apply first a shear strain followed by a volumestrain or vice versa. In the following, we specify explicitly the pathsthat we follow and check the dependency of the final outcome on thechoices of paths.

Now, let us start our analysis by considering what happens fol-lowing a simple cyclic deformation: First, the system is strained normally(0, 0)→ (D, 0), then sheared (D, 0)→ (D, g), and lastly sheared back in the

Jin et al., Sci. Adv. 2018;4 : eaat6387 7 December 2018

reversed way (D, g) → (D, 0). The following three typical behaviors arefound: The response of the glass can be reversible, partially irreversible,or totally irreversible, which signals stable, marginally stable, and un-stable states of the glass. Typical examples of the stress-strain curvesare shown in Fig. 1.

(i) Reversible regime: For small g, the stress s increases smoothlyand monotonically with increasing g (green lines in Fig. 1, A and D).To the first order, the stress is linear, ds = mdg, where m is the shearmodulus. If the strain is releasedwith� :

g, the stress-strain curve reversesto the origin—this is a typical elastic response.

(ii) Partially irreversible regime: For larger g above a certain thresh-old gG , the stress-strain curve becomes jerky, consisting of piecewiselinear elastic responses followed by small but abrupt stress drops (redlines in Fig. 1, A andD). Each stress drop corresponds to a plastic event,where some particles rearrange their positions. The glass in this regimeis marginally stable in the sense that a tiny dg could make the systemunstable by triggering these plastic events, but the particles immediatelyfind another stable configuration nearby, avoiding further failure of theentire system. Although the stress-strain curve is locally irreversible forsmall reversed strain, globally, it eventually returns to the origin whenthe shear strain is released back to g = 0 (the red lines in Fig. 1, A andD,merge with the green lines below gG). We call this behavior partialirreversibility.

(iii) Limit of existence of the solid: For even larger g, the glass facestwo kinds of consequences depending on the volume strain D appliedbefore shearing.

• Yielding:At the yielding strain gY, a sudden andnotable stress dropoccurs. When this happens, the entire system breaks into two piecesthat can slide with respect to each other along a fracture. As shownby the stress-strain curve (black line in Fig. 1A), yielding is ir-reversible—once the glass is broken, it cannot be “repaired.” In a con-stant volume protocol where we keep the total volume of the systemunchanged, yielding can be seen only if the system is not compressedto too high packing fractions, i.e., for not too negative volume strain D.

• Shear jamming: The behavior changes markedly if the system iscompressed more before shearing. In this case, the system jams at theshear jamming strain gJ, which is signaled by the divergence of the shearstress (black line in Fig. 1D).

To examine the reversibility more carefully, we measure the relativemean squared displacement Dr (see Materials and Methods for thedefinition) between the initial state at g = 0 before the shear is appliedand the final state at g = 0 after a single cycle of shear is applied (Fig. 1, Band E). If the initial and the final configurations are identical, Dr = 0;otherwise, the more different they are, the larger Dr is. The value ofDr returns to zero in the reversible and partially irreversible cases butbecomes nonzero in the irreversible case, being consistent with theabove analysis based on the stress-strain curves. Note that, here, we ne-glect differences on the microscopic scale of vibrational cage size D ≲0.01 (seeMaterials andMethods), i.e., a system is called irreversible onlyif the difference on Dr between the initial and final configurations islarger than D. We have also examined that the above behaviors persistin multicycle shears (see fig. S2).

It is useful to understand our observations using a schematic pictureof the free-energy landscape. Each glass state is represented by a basin offree-energy F(φg; D, g; N), which is distorted upon increasing shearstrain g (Fig. 1, C and F). The shear stress is nothing but the slope of

the free-energy sðφg; D; g;NÞ ¼ bN

∂Fðφg ;D;g;NÞ∂g , with b being the inverse

temperature. The associated shear modulus is obtained by taking one

3 of 12

SC I ENCE ADVANCES | R E S EARCH ART I C L E

on March 29, 2020

http://advances.sciencemag.org/

Dow

nloaded from

more derivative with respect to g, which gives nothing but the curvatureof the free-energy basin. In the stable regime, the basin is smooth; in themarginally stable regime, the basin becomes rough, consisting of manysub-basins with larger associated shear modulus, which results in thefailure of pure elasticity (33, 36, 37). In this state, the system can releasethe stress via hopping between different sub-basins, corresponding toplastic events, which leads to emergent slow relaxation of shear stress(24, 37). For very large strains, the system either yields by escaping fromthe glass basin (Fig. 1C) or jams by hitting the vertical wall due to thehard-core constraint (Fig. 1F).

The plastic behavior appearing in the partially irreversible regimetakes place at mesoscopic scales, and it would be averaged out in amac-roscopic system at large enough time scales (37). There is evidencewhich shows that the minimum strain increment dgtrigger(N) to triggera plastic event vanishes in the thermodynamic limit N → ∞ (33, 42).This implies that in a macroscopic system, any small but finite incre-ment of strain would cause a nonzero number of mesoscopic plasticevents (11). Moreover, time-dependent aging effects associated to theseplastic events were observed in stress relaxations (24). Therefore, inmacroscopic systems at large enough time scales, the plasticity wouldbe averaged out, and one would observe just a renormalized “elastic”response. The bare elastic response can only be seen within the piece-wise linear mesoscopic response for dg < dgtrigger(N). This means that

Jin et al., Sci. Adv. 2018;4 : eaat6387 7 December 2018

two different shearmoduli can be defined: the bare one mbare = limN→ ∞

limdg → 0ds(φg; D, g; N)/dg that takes into account the piecewise elasticbehavior between two subsequent avalanches, and themacroscopic onemmacro = limdg → 0limN → ∞ds(φg; D, g; N)/dg, which represent the av-erage behavior and is smaller than the former (33, 37). Therefore, thesmall strain dg→ 0 limit and the thermodynamics limit do not commutein the marginal plastic phase (see text S1 for a detailed discussion).

Stability-reversibility map and G-EOSThese three different kinds of responses of the system to simple cyclicshear, listed above as (i) to (iii), can be summarized by the stability-reversibility map in the D − g plane, as shown in Fig. 2. There we alsoshow a typical plastic event in the marginal phase (Fig. 2B) and ayielding event (Fig. 2C), which indicate two different mechanismsthat can cause a failure of stability. As long as the glass remains stableor marginally stable, its macroscopic properties can be characterized bythe G-EOS for the pressure p = pglass(φg; D, g) and the shear stress s =sglass(φg; D, g), as shown in Fig. 3 (A andB). The pressure p and the shearstresss are derivatives of the glass free-energy− bF(φg; D, g) with respectto D and g, respectively.

Along the g = 0 line, the evolution of the systemunder volume strainD will eventually lead the system to either jamming after sufficient com-pression D < 0 or melting after sufficient decompression D > 0. At

= −0.0069

= −0.029

C

γγYγG

F

F F

γγJγG

BA γG γY

0 0.05 0.1 0.15 0.2−10

0

10

20

30

γ

σ

0 0.05 0.1 0.15 0.2

0

0.5

1

1.5

2

γ

r

ED

γG γJ

0 0.05 0.1 0.150

50

100

150

200

250

γ

σ

0 0.05 0.1 0.15

0

0.2

0.4

0.6

0.8

γ

r

0 0.05 0.10

100

200

Fig. 1. Reversibility, partial irreversiblity, and irreversiblity of the HS glass under simple shear. Here, we display typical behaviors of a glass sample obtained by annealingup toϕg = 0.655. (A) Single-realization stress-strain curve of a glass at the fixed volume strain D=−0.0069 (ϕ= 0.66). The shear strain is reversed at g= 0.06 (green), 0.14 (red),and 0.2 (black). The smooth and jerky regimes are separated by gG ~ 0.09. The yielding strain gY ~ 0.144 is also indicated. (B) Corresponding plot of the relativemean squareddisplacementDr as a function of g. (C) Schematic illustration of the free-energy glass basin under shear. (D to F) The sameas (A) to (C) but at volume strain D =−0.029 (ϕ=0.675) forwhich gG ~ 0.073 and gJ ~ 0.14. In the inset in (D), five different realizations for the same sample are plotted, showing that plastic avalanches only occur above gG. See fig. S1 for thecase D = 0.057 (ϕ = 0.62) for which the systemdoes not go through the partially irreversible regime under shear up to the yielding. The three cases (D = −0.0069, −0.029, 0.057) areindicated by black arrows in the stability-reversibility map in Fig. 2.

4 of 12

SC I ENCE ADVANCES | R E S EARCH ART I C L E

on March 29, 2020

http://advances.sciencemag.org/

Dow

nloaded from

jamming, particles form an isostatic rigid contact network such that nofurther compression can be applied. Decompressing the system reducesp, which eventuallymelts the system into a liquid state. The evolution ofthe pressure p follows the zero–shear strain G-EOS p = pglass(φg; D, 0)both upon compression and decompression. Obviously, s = sglass(φg; D,0) = 0.

Applying a shear strain at any point on the g = 0 G-EOSs p =pglass(φg; D, 0) and s = sglass(φg; D, 0) allows us to explore the volumestrain versus shear strain phase diagram, andwe can track both the pres-sure p = pglass(φg; D, g) and the stress s = sglass(φg; D, g). Under shear, theglass has two possible fates: either it yields across the shear yieldingline g = gY(φg; D) or it jams at the shear jamming line g = gJ(φg; D).Yielding can be detected by analyzing the stress-strain curve, i.e.,sglass(φg; D, g) versusg,while shear jamming is signaledby adivergenceofboth the pressure pglass(φg; D, g)→∞ and the stress sglass(φg; D, g)→∞as g→ gJ(φg; D). The shear yielding and the shear jamming lines de-fine the boundaries of the stability of the HS glass, beyond which theglass is unstable or simply forbidden. The two lines meet at a yielding-jamming crossover point [Dc(φg), gc(φg)] or [φc(φg), gc(φg)].

Within the boundary of the stability-reversibility map, there are twophases: the stable (reversible) phase and the marginally stable (partiallyirreversible) phase. We call the line that separates the two a Gardnerline. Across this line, the qualitative nature of the system’s responseto deformations changes: The stress-strain curve is smooth within thestable (reversible) phase but jerky in the marginally stable (partiallyirreversible) phase. The stability-reversibility map shown in Fig. 2 sug-

Jin et al., Sci. Adv. 2018;4 : eaat6387 7 December 2018

gests that if we choose an D such that the Gardner line is not crossedalong the path (D, 0)→ (D, gY), then no marginally stable region shouldbe observed. Figure S1 shows such a case (with D = 0.057) where we donot observe partial irreversibility all the way up to yielding. The termGardner line is inferred from the MF glass theory (5, 29), in which acontinuous phase transition, the Gardner transition, occurs on this line.However, whether it is a genuine transition line or a crossover line inthree dimensions is an open question, as we noted in the Introduction.In the next subsection, wewill explain howwe estimate this line numer-ically in the present system.

We made the choice in Fig. 2 to represent the stability-reversibilitymap in terms of strains (volume and shear). In fig. S3A, we plot it interms of volume fraction φ and shear strain g, which can be directlycompared with the theoretical prediction in (29). In some experiments,the shear stress is controlled instead of the shear strain, and in that case,it is customary to represent the phase diagram in the density-stressplane. Such a figure is reported in fig. S3B, which is directly comparableto the phase diagram reported in the granular experiment of (30).

The stability-reversibility map and the G-EOS depend on the prep-aration density φg of the glass, which represents the depth of annealing.As shown in Fig. 3C, where the G-EOS and L-EOS are displayedtogether, the g = 0 G-EOS and the L-EOS intersect at the point (φ, g) =(φg, 0), which shows the intrinsic connection betweenG-EOS and L-EOS.The initial unperturbed glass is located at (D, g) = (0, 0) in the stability-reversibility map.

Marginal stability and partial irreversibilityHaving presented above our most important results, in the following,we show more details on how the stability-reversibility map and theG-EOS are obtained in our numerical experiments. To this end, ateach φg, we prepare Ns = 100 independent equilibrium supercooledliquid configurations by the swap algorithm, which have different equi-librium positions of particles and are called samples. By switching offthe swap, they become glasses. For each sample of glass, we repeat Nr ~50 − 200 realizations of a given protocol, which is a combination of com-pression (or decompression) and simple shear. Each realization startsfrom statistically independent initial particle velocities drawn from theMaxwell-Boltzmann distribution at φg.

TheGardner transitionmarks the point where the elastic behavior isreplaced by a partially plastic one. Avalanches and plasticity are ex-tremely marked in finite size systems, while they are averaged out onmacroscopic length and time scales. Furthermore, in finite size systems,even though each individual stress-strain curve is jerky in the marginalphase as shown in Fig. 1, the average over different samples and realiza-tions washes out all the sudden drops, giving rise to a smooth profile.Therefore, macroscopic G-EOSs by themselves do not allow the de-tection of the marginally stable phase (see text S1 and fig. S4 for adetailed discussion). To precisely locate the onset of plasticity and themarginal phase, we will examine the hysteretic response to very smallshear increments.

Inspired from spin glass experiments (43), we compare the shearstressmeasured by two different protocols, the so-called zero-field com-pression (ZFC) and the field compression (FC) protocols (24). Withinthe FC protocol, one first compresses the system and then shears it. Inthe ZFC, one instead reverses the order (see Materials andMethods formore details). The FC stresssFC can be considered as the large time limitof sZFC, as long as the yielding and the a-relaxation do not occur (24, 37).For elastic solids such as crystals, the two stresses are identical. Formarginally stable glasses, however, sFC is lower than sZFC, because of

A

C

B

mar

gina

l

−0.05 0 0.05 0.1 0.15 0.2 0.250

0.05

0.1

0.15

0.2

γ

Fig. 2. Stability-reversibility map. (A) Stability-reversibility map of the HS glass an-nealed up toϕg = 0.655, obtained by the constant pressure−shear (CP-S) protocol (seeMaterials andMethods for the definition). The horizontal axis is the volume strain D, andthe vertical axis is the shear strain g. The origin (0, 0) marked by the green square re-presents the initial glass without deformations. The glass remains stable only inside aregion bounded by the yielding line gY(ϕg; D) (brown diamonds) and the shearjamming line gJ(ϕg; D) (blue triangles). The shear yielding and the shear jamming linesmeet at the yielding-jamming crossover point (gray pentagon) (Dc, gc) = (−0.020(4),0.16(1)) (corresponding to ϕc = 0.669(3)). The Gardner line gG(ϕg; D, g) (red circles)separates the marginally stable glass phase (blue area) from the stable glass phase(yellow area). Under decompression, i.e., increasing Dwith g = 0, the glass becomesfully liquefied at the melting point (pink cross). In the plot, the stable, marginallystable, and unstable regimes correspond to reversible, partially irreversible, and ir-reversible regimes, respectively. The black arrows at the bottom indicate the vol-ume strains used in Fig. 1 (the two arrows on the left of the green square at D =−0.0069and D = −0.029, which are above and below Dc, respectively) and fig. S1 (the arrow onthe right at D = 0.057). (B) The snapshot shows the particles involved in a typical plasticevent in the marginally stable glass phase. (C) The snapshot shows the planar fracturestructure that appears during yielding. The colors in (B) and (C) represent the relative

single-particle displacement dir ¼ffiffiffiffiffiDir

q; warmer colors indicate higher values.

5 of 12

SC I ENCE ADVANCES | R E S EARCH ART I C L E

on March 29, 2020

http://advances.sciencemag.org/

Dow

nloaded from

the stress relaxation associated to the plastic events happening at me-soscopic scales. The origin of two responses can be attributed to theorganization of free-energy landscape shown schematically in Fig. 1 (Cand F). Roughly speaking, the ZFC stress sZFC is dominated by theshort time response within the small sub-basins, while the FC stresssFC reflects the renormalized, long time response within the big en-velope of sub-basins. The bifurcation point between the two stressesdetermines the Gardner point. Note that this criterion to determinethe Gardner point is the same as the one used in (24). Figure 4A showsthe data used to obtain the Gardner points DG(φg; g) for a few differentvalues of g. Connecting theGardner points gives theGardner line g = gG(φg; D) in Fig. 2. See fig. S5 for the same results obtained for othervalues of φg.

Alternatively, one may look at caging order parameters such as themean squared displacement D and the typical separation between tworeplicas DAB (23) (see Materials and Methods for more precise defini-tions). The two replicas are generated from the same initial sample intwo independent realizations. They are first compressed to a target Dunder zero shear strain and then sheared to the target shear strain gunder the fixed D. When the Gardner point gG(φg; D) is crossed over,D andDAB should also separate.However, this is a sign of critical behavior

only if the corresponding susceptibility cAB ¼ N ⟨D2AB⟩�⟨DAB⟩

2

⟨DAB⟩2grows (39).

Here, ⟨… ⟩ represents the average over both samples and realizations.cABis a spin glass–like susceptibility whose growth suggests the increase ofheterogeneity and cooperativity in the system, as suggested by the MFtheory (5). The behavior of cAB can be inferred from Fig. 1B, where weplot the probability distribution P(DAB) of DAB. We see a Gaussian-likebehavior below the Gardner threshold, fat tailed around it, and doublepeaked above it. The Gardner point inferred in this way gG(φg = 0.655;

Jin et al., Sci. Adv. 2018;4 : eaat6387 7 December 2018

D = −0.036) ≈ 0.06 is consistent with the determination from ZFC-FCprotocols DG(φg = 0.655; g = 0.06) ≈ −0.036.

This result provides a strong evidence that partial irreversibility andplasticity in Fig. 1 are essentially related to emerging marginal stability.We perform the following test to examine their connections more di-rectly. Starting from a compressed glass at (D, g = 0), we first shear theglass to a target shear strain at (D, g − dg) under constant volume andthen apply an additional cycle of small shear strain dg = 0.004, followingthe path (D, g − dg)→ (D, g) → (D, g − dg). If the system is reversible,then the difference between the stresses before and after the single cyclicshear, ds1 ¼ ðsbefore � safterÞ=sbefore, should be zero, otherwise not.Figure 4C confirms that ds1ðgÞ begins to grow around the gG esti-mated from the other two approaches described before (Fig. 4, A andB). However, this kind of irreversibility is only partial because the sys-tem is reversible under a circle of shear with larger strain. Systems fol-lowing the path (D, dg)→ (D, g)→ (D, dg), where dg = 0.004 is fixed andg is varying, show that the stress difference ds2 is nearly zero for any g.

Last, it is important to stress that in our three-dimensional numer-ical simulations, as in previous ones (23, 24), we cannot decide onwhether the separation between the stable and marginally stable phasecorresponds to a true phase transition. This would require, for instance,a careful study of finite size effects on cAB to extract the behavior forN→∞, which is very difficult already in much simpler models suchas spin glasses. The focus of our work is on relating the Gardner line,which is only a (quite sharp) crossover in our simulations, to theonset of partial irreversibility.

Shear yielding and shear jammingUp to now we have investigated the interior of the stability-reversibilitymap. Next, we turn to explore the boundaries of the stability-reversibility

γ

A

γ

B

/ϕ

1.41.5

1.61.7

1.81.9

γ

0

0.05

0.1

0.15

0.20

0.02

0.04

0.06

0.08

00.0200.020.040.060.08

C

1/p

1/p

Log10

/pFig. 3. Glass EOS. (A and B) We show the G-EOSs for the pressure p = pglass(ϕg; D, g) and shear stress s = sglass(ϕg; D, g) for the HS glass prepared at density ϕg = 0.655 by heatmaps. The color bar scales represent 1/p and log10(1/s). The thin black lines represent isobaric (constant-p) lines for p= 14.5, 15.0, 15.8, 16.5, 17, 18, 19, 21, 27, 40, 65, 160, and 1000(from right to left) in (A) and constant-s lines for s = 0.3, 1, 3, 10, 30, 100 (from right to left) in (B). The data are obtained via the CP-S protocol (see Materials and Methods for thedefinition). (C) Three-dimensional view of the same G-EOS for the pressure (colored plane) and the L-EOS p = pliq(ϕ) (green line). Here, specific volume 1/ϕ is used instead of thevolume strain D. The evolution of liquid under compression/decompression follows the Carnahan-Stirling empirical L-EOS (23). The golden star represents the mode-couplingtheory (MCT) transition point, which is obtained from extrapolation of the relaxation time according to the MCT scaling (23). Note that pglass(ϕg; 0, 0) = pliq(ϕg) holds by thedefinition of ϕg. See Fig. 2 for the meaning of symbols and fig. S9 for the cases of other ϕg and other exploration protocols.

6 of 12

SC I ENCE ADVANCES | R E S EARCH ART I C L E

on March 29, 2020

http://advances.sciencemag.org/

Dow

nloaded from

map by analyzing the G-EOSs both in pressure and shear stress. Fromnow on, all data presented are averaged over different samples and real-izations. Therefore, even with a finite size system, the individual plasticevents will be averaged out. Furthermore, we will plot the G-EOSs on aphase diagramusing 1/φ (instead of, equivalently, D) and g to better showtheir relations to L-EOS.

First of all, starting froman equilibriumconfiguration at (φ, g) = (φg, 0)or (D, g) = (0, 0), the system melts under decompression for sufficientlylarge D. We define the melting point as the crossover point betweenthe g = 0 G-EOS for the pressure and the L-EOS (see Figs. 3C and 5G).Themelting point sets the upper bound of the stability-reversibilitymapalong the g = 0 line.

To systematically explore the stability-reversibility map, we designthree specific protocols combining compression/decompression andshear, namely, CP-S, CV-S, and CS-C/D (see Materials and Methodsfor details). These protocols can be realized also in experiments. In prin-ciple, the EOS should not be protocol dependent, but whether it is alsothe case for G-EOS is not so obvious.

In the CP-S protocol, for any fixed pressure p, the specific volume1/φ (or volume strain D) evolves with shear strain g, which defines aG-EOS for the pressure. Figure 5A shows theG-EOSs for a few differentpressures p in a g − 1/φ plot. Such a plot is essentially the projection ofthe three-dimensional plot of theG-EOSs for the pressure p= p(φg; D, g)in Fig. 3C onto the g − 1/φ plane. The data show that the specific volume1/φ expands as strain g is increased, known as the dilatancy effect. Thedilatancy is stronger for better annealed glasses, as observed previouslyin (24), and at lower pressure for a fixed quality of annealing, as shownhere. Both observations are consistent with theoretical predictions [ Fig. 2in (22) and Fig. 2A in (29), respectively]. Note that this dilatancy effectshall be distinguished from the one discussed in the context of steadyflow,which is necessarily correlated to friction, as shown in (44). At highpressures, the isobaric lines are nearly parallel to the shear jamming line,which corresponds to the p = ∞ isobaric line by the definition of jam-ming. On the other hand, the average stress s shown in Fig. 5B initiallyincreases with the shear strain, but it eventually approaches a plateauafter a big drop corresponding to yielding.We define the yielding pointas the peak of the stress susceptibility cs = N(⟨s2⟩ − ⟨s⟩2) (see Fig. 5C).The yielding point is approximately at the middle of the drop on thestress-strain curve, corresponding to the steepest decrease of stress.After yielding, the shear stress generally remains nonzero, indicatingthat the glass is not completely fluidized. Real-space visualization showsthat the glass breaks into two pieces sliding against each other (see

Jin et al., Sci. Adv. 2018;4 : eaat6387 7 December 2018

Fig. 2C). However, near themelting point, such a picturemight change,because melting could mix with yielding, giving rise to a hybrid be-havior. We will not discuss this situation in detail here. By connectingthe yielding strains obtained at different p, we obtain the yielding line.We notice that for a certain range of pressure p near pg of the initialglass, the yielding strain g*Y ≈ 0:118 is nearly independent of p.

In Fig. 5 (D and E), we show how the inverse pressure 1/p and shearstress s evolve with g for various φ in the CV-S protocol. We find athreshold density φc (see fig. S6 for how φc is determined), whichseparates the shear yielding and shear jamming cases. If φ < φc, the sys-tem generally yields at large g; otherwise, both pressure and shear stressdiverge as g is increased, indicating shear jamming. In this protocol, theyielding point can be determined again from the peak of the stress sus-ceptibility (see Fig. 5F). In the shear jamming case, the pressure and shearstress both follow the free-volume scaling laws: p ~ (gJ − g)−1 and s ~(gJ − g)−1 (see fig. S7). The shear jamming is a natural consequence ofthe dilatancy effect (i.e., p increases with g for fixed φ), as long as thesystem does not yield. Thus, φc results from the competition betweenthe dilatancy effect and the tendency to break the system at large strains.We have checked that all the shear-jammed packings that we createsatisfy the isostatic condition (45), i.e., the average coordination numberZ = 6, once the ratters (particles that have less than four contacts) areexcluded, and that the shear jamming transition falls in the same uni-versality class of the usual jamming transition in the absence of shear.

Figure 5 (G and H) shows the constant-g EOSs of the pressure andshear stress for a few different g in the CS-C/D protocol. For small shearstrains, g < g*Y, the system jams at a g-dependent jamming density φJunder compression. For shear strains larger than the yielding straing >g*Y, however, the G-EOSs for pressure collapse onto the same curve, andconsequently, the jamming density φJ also does not change with ganymore. This observation is consistentwith our interpretation of yieldedstates: The glass just breaks into two pieces of solids at g*Y by forming aplanar fracture. These planar structures should haveminor effect on bulkproperties like the pressure. On the other hand, the glass always meltsunder decompression, for any g. We find that the melting point isindependent of g, both below and above g*Y. The stress susceptibilitycs displays a peak upon decompression, which reveals the vestige ofyielding, and therefore can be used to define the yielding point in theCS-C/D protocol (Fig. 5I). For g < g*Y, the yielding density φ increaseswith g; for g > g*Y, the peak does not exist anymore, and the yieldingpoint cannot be defined as expected. In addition, we show and discussthe behavior of the pressure susceptibility cp in fig. S8.

CBA

−0.06 −0.04 −0.02 0 0.02 0.04

0

0.002

0.004

0.006

0.008

0.01

ZFC−

FC

γ = 0γ = 0.02γ = 0.04γ = 0.06γ = 0.08γ = 0.1

10 4 10 3 10 210 1

100

101

102

103

104

P

0 0.02 0.04 0.06 0.08 0.1

0

0.01

0.02

0.03

γ

Fig. 4. Marginal stability andpartial irreversiblity. (A) Difference between ZFC and FC stresses (rescaled by p,~s ¼ s=p) as a functionof the volume strain D, forϕg = 0.655 anda fewdifferently fixed g. The Gardner threshold DG(ϕg; g) is determined as the point where this difference exceeds 0.0006 (horizontal dashed line). For example, the vertical dashedline marks DG(ϕg = 0.655; g = 0.06) ≈ −0.036. (B) Distribution of DAB over samples and realizations, at fixed volume strain D = −0.036 (or ϕ = 0.68), for different g. From the data, weestimate gG(ϕg = 0.655; D = −0.036) ≈ 0.06, where P(DAB) becomes non-Gaussian (green points), consistingwith (A). (C) The stress dropsds1 andds2 measured in single cycle shearsimulations are plotted as functions of g at fixed D = −0.036 (see the text for the definitions). The vertical dashed line represents gG(ϕg = 0.655; D = −0.036) ≈ 0.06 estimated in (A)and (B). Note that at D = −0.036, the system jams under constant volume shear (see Fig. 2) so that we can exclude any irreversibility caused by yielding.

7 of 12

SC I ENCE ADVANCES | R E S EARCH ART I C L E

on March 29, 2020

http://advances.sciencemag.org/

Dow

nloaded from

Dependence on protocols and system sizesLet us discuss how the stability-reversibility map and G-EOSs dependon protocols. There are two important sources of protocol dependences.First, the stability-reversibilitymap and theG-EOSs depend on the glasstransition point φg, and φg itself depends on the protocol parameterssuch as the compression rate in a standard compression annealingprotocol (here, it is a function of where we stop swap moves). Figure 6Ashows the stability-reversibility maps for three different φg, correspond-ing to three typical experimental time scales as discussed previously (seefig. S9A for the three-dimensional representations). They share com-mon qualitative features in general. The stable regime expands with

Jin et al., Sci. Adv. 2018;4 : eaat6387 7 December 2018

φg, as one would naturally expect that more deeply annealed glassesshould be more stable. The shear jamming line becomes more verticalwith decreasingφg. This trend is consistent with previous numerical ob-servations, which show that, in the thermodynamical limit, the shearjamming line is completely vertical for infinitely rapidly quenchedsystems (46).Moreover, we point out that the Gardner transition pointscannot be determined unambiguously using our approaches for the lessannealed systems φg = 0.631, g > 0.06 and φg = 0.609, g > 0 (see fig. S5)because different activated dynamics, such as plastic rearrangements,formation of fractured structures, and a-relaxations cannot be wellseparated.

A

B

C

D

E

F

G

H

I

1.4 1.5 1.6 1.7 1.8 1.90

0.05

0.1

0.15

0.2γ

0 0.05 0.1 0.15 0.20

0.02

0.04

0.06

0.08

γ

/p

1.4 1.5 1.6 1.7 1.8 1.90

0.02

0.04

0.06

0.08

/p = 0

= 0 02

= 0 04

= 0 06

= 0 08

= 0 1

= 0 118

0 0.05 0.1 0.15 0.210 2

10 1

100

101

102

103

γ

σ

0 0.05 0.1 0.15 0.210 2

10 1

100

101

102

103

104

γ

σ

1.4 1.5 1.6 1.7 1.8 1.910 3

10 2

10 1

100

101

102

103

104

σ

0 0.05 0.1 0.15 0.2100

101

102

103

104

105

106

107

γ0 0.05 0.1 0.15 0.2

101

102

103

104

105

106

γ1.7 1.8 1.910 2

10 1

100

101

/

/p2

ϕ

Fig. 5. Yielding, shear jamming, andmelting in CP-S, CV-S, and CS-C/D protocols. (A to C) G-EOSs obtained by the CP-S protocol for the ϕg = 0.655 system. The solid thinlines are isobaric lines for p=14.5, 15.0, 15.8, 16.5, 17, 18, 19, 21, 27, 40, 65, 160, 1000 [from right to left in (A); the same colors are used for (B) and (C)]. The yielding line (filled browndiamonds) for the CP-S protocol is determined from the peak positions of the stress susceptibility-strain (cs − g) curves shown in (C). (D to F) G-EOSs obtained by the constantvolume–shear (CV-S) protocol. The solid thin lines are isochoric (constant-ϕ) lines for ϕ = 0.558, 0.562, 0.568, 0.574, 0.579, 0.586, 0.595, 0.607, 0.616, 0.635, 0.655, 0.667, where thesystem exhibits yielding [from bottom to top in (E)]. The dashed thin lines are isochoric lines for ϕ = 0.669, 0.676, 0.679, 0.684, 0.687, 0.689, 0.692, 0.693, 0.695, where the systemexhibits shear jamming [from right to left in (E)]. The yielding line (open brown diamonds) for the CV-S protocol is determined from the peak positions on the cs − g curves shownin (F). (G to I) G-EOSs obtained by the constant shear strain–compression/decompression (CS-C/D) protocol. The solid (decompression) and dashed (compression) thin linesrepresent constant-g lines. The melting point (pink cross) is defined as the intersection between G-EOSs and L-EOS [thick green line in (G)]. The half-filled brown diamondsare the yielding line for the CS-C/D protocol determined from the peak positions on the cs − g curves shown in (I). See Fig. 2 for the meaning of other symbols.

8 of 12

SC I ENCE ADVANCES | R E S EARCH ART I C L E

on March 29, 2020

http://advances.sciencemag.org/

Dow

nloaded from

Second, we show in Fig. 6B how the stability-reversibility map andalso the G-EOSs for the pressure depend on the exploration pro-tocols (CP-S, CV-S, and CS-C/D); see fig. S9 (B and C) for the three-dimensional representations. We find a protocol-independent regimeðD < D*; g < g*YÞ, where all three protocols give the same pressure.The part of the stability-reversibility map above g*Y cannot be accessedby the CS-C/D protocol. For D > D*, the yielding line bends down dif-ferently, depending on the protocol. The system yieldsmost easily in theCV-S protocol, presumably because the liquid bubbles formed aroundmelting are easier to expand in a volume-controlled protocol (40).

Last, we discuss briefly how the stability-reversibility maps dependon the system size N in fig. S10. We do not observe appreciable finitesize effects on the shear jamming line. On the other hand, the yieldingline exhibits strong finite size effects, but we expect it to converge atlarger sizes, based on the recent results of (9). Using the presentmethods,we also do not find strongN dependence on the Gardner line, consistentwith the data in (24). However, we stress that based on available nu-merical results, we cannot conclude on the thermodynamic behaviorof the Gardner transition. Understanding whether it is a sharp transitionor a crossover is an active and hot topic in the field, through numerical(23), experimental (31), and theoretical analyses (39, 47–49). While thefinite size analysis presented here shall not be considered conclusive, weleave a more detailed finite size study on yielding, shear jamming, andthe Gardner transition for future work.

DISCUSSIONHere, we investigate the stability and the reversibility of polydisperseHSglasses under volume and shear strains. We prepare equilibrium super-cooled liquid states, with different degrees of stability ranging froma fastquench to an extremely slow annealing, corresponding to ultrastableconfigurations. Each configuration corresponds to a glass within a timescale that is shorter than the structural relaxation time. We study thestability of the glass under volume and shear strains and find that theregion of stability is delimited by lines where the system can either yieldor jam.We also find that within the region of stability, the system can beeither a normal solid, which essentially responds elastically and re-versibly to perturbations, or a marginally stable solid, which respondsplastically and in a partially irreversible way. More precisely, the mainoutcomes of our analysis are the following:

1) Response. The response of the system to a shear strain is eitherpurely elastic, partially plastic, or fully plastic (yielding), depending on

Jin et al., Sci. Adv. 2018;4 : eaat6387 7 December 2018

the quality of annealing and the amount of volume and shear strainsimposed to it.

2) Failure. Well-annealed glasses (large φg), when sheared at suffi-ciently low densities (large volume strain D), behave purely elastically upto yielding, which is an abrupt process where a fracture is formed andthe glass fails. At higher densities, they display a partial plastic phasebefore yielding is reached. At even higher densities, they display shearjamming (under constant volume shear). The shear yielding and shearjamming lines delimit the region of existence of the HS amorphous solid.

3) Marginality. Along the solid part of the stress-strain curves, thepartial plastic behavior is well separated from the purely elastic one bythe Gardner point. The onset of partial plasticity is accompanied by theemergence of critical behavior andmarginal stability. Beyond theGardnerpoint, the shearmodulus of the systembecomes history dependent. At thesame time, a growing spin glass–like susceptibility is observed.

4) Reversibility. The purely elastic phase is globally reversible: Oncethe shear is released, the system gets back to the original configuration.The partially plastic marginal glass phase is partially irreversible: Uponreleasing the deformation by a small amount, the system is not able toget back to the previous state, while upon complete release, the system isable to get back to the original configuration. Yielding corresponds tocomplete irreversibility: Once broken, the system starts to flow, and it isnot able to get back to the original configuration once the strain is com-pletely released.

By collecting together the boundaries of the different regions, we ob-tained a complete stability-reversibility map (phase diagram), reportedin Fig. 2. The stability-reversibilitymap obtained in the present study forthree-dimensional HS glasses can be compared with the one obtainedby the MF theory in the large dimensional limit (29). The most impor-tant features, such as the presence of the shear jamming and the shearyielding lines that delimit the stability region and the presence of theGardner line, are qualitatively in good agreement with the predictionsof the theory. There are, however, several important differences. (i) Theshear yielding line in the three-dimensional system is not a spinodalline, as predicted by theMF theory (22). The abrupt formation of a frac-ture is completelymissed by theMF theory, which does not describe thespatial fluctuations of stress that accumulate around the fracture. (ii)The point (Dc, gc) where the shear yielding and the shear jamming linesmeet is predicted to be a critical point in theMF theory, but it is rather acrossover point in the three-dimensional system. (iii) The marginallystable phase has larger gY than the stable phase. This suggests thatthe plastic events in the marginal phase help the system to avoid total

-0.1 -0.05 0 0.05 0.1 0.15 0.20

0.05

0.1

0.15

0.2

γ

A B

−0.1 −0.05 0 0.05 0.1 0.15 0.2 0.250

0.05

0.1

0.15

0.2

γ

0.25-0.002

0

0.002

0.004

0.006

0.008

Fig. 6. Protocol dependence of the stability-reversibility map. (A) Stability-reversibility maps for ϕg = 0.609 (blue), 0.631 (red), 0.655 (black). (B) Stability-reversibilitymaps obtained in three different protocols (CP-S, CV-S, and CS-C/D). The color bar indicates the difference on 1/p between the CS-C/D and the CP-S protocols. Thehorizontal and vertical lines represent g�Y ≈ 0:118 and D* ≈ 0.1. See Figs. 2 and 5 for the meaning of symbols.

9 of 12

SC I ENCE ADVANCES | R E S EARCH ART I C L E

on March 29, 2020

http://advances.sciencemag.org/

Dow

nloaded from

failure. In the theory, the shear yielding line bends down rather thanbends up near the point (Dc, gc) [see Fig. 3 of (29)].

Note that the MF predictions of (29) were obtained using the so-called replica symmetric (RS) ansatz. To properly consider yielding inthe marginally stable phase, one should extend the computation to afull-step RS breaking (fullRSB) ansatz (50). This might help in solvingsome of the discrepancies between the analytical and the numericalresults. According to theRS theory, yielding is a spinodal transitionwithdisorder (22). However, it is not clear how this picture will be modifiedby a fullRSB theory.

Our simulation results show that a well-annealed glass (φg wellabove the MCT density φMCT) yields abruptly—it is brittle. However,a poorly annealed glass (φg ~φMCT)may instead continuously yield intoa plastic flow state (10, 12)—it is more ductile. We expect that near themelting point, even a well-annealed glass would behave similarly to apoorly annealed one, as it would become much “softer” upon de-compression. Nevertheless, the yielding point can be determined fromthe peak of cs for both cases as shownhere.Our approach thus providesa unified framework to study the transition between the two distinctmechanisms of yielding. The possibility of two yielding mechanismsismissed by the currentMF theory. A dynamical extension ofMFmightaccount for these effects. Understanding the nature of the yieldingtransition (51–53) is a crucial problem that requires further analysis.

The plastic events we observe in the partially irreversible phase couldcorrespond to two different types of soft modes: collective modes, as-sociated to a diverging length scale, as predicted by the MF theory inthe marginally stable phase (5, 11), or localized modes, such as the onesthat have been observed in numerical studies of low-dimensionalsystems (54–56). In this study, we did not investigate systematicallythe nature of the plastic events in our system, but the growth of the spinglass–like susceptibility in our data suggests the presence, in our HSmodel, of large-scale collective excitations. Note that the situation couldbe radically different in soft potential models (38, 55, 56). We also stressthat while the existence of partial plasticity before yielding is well known(6–8), our well-annealed systems provide an example where the pureelasticity and partial plasticity regimes are well separated, allowing usto define a line (the Gardner line) that separates them in the stability-reversibility map.

Last, concerning the reversibility, here we focus on the reversibilitywith respect to just one cycle of simple shear (see fig. S2 for the resultsunder a few cycles). In cyclic shear protocols, a steady state can be reachedaftermany cycles (17, 57). Very complicated dynamics should be involvedin theseprocesses. Itwouldbe interesting to systematically extend thepres-ent study to multiple cyclic shear to understand better these processes.

MATERIALS AND METHODSModelThe system consists of N = 1000 (unless otherwise specified) HS parti-cles with a diameter distribution P(D) ~D−3, forDmin≤D≤Dmin/0.45.The continuous polydispersity was sufficient to suppress crystallizationeven in deep annealing and optimized the efficiency of swap algorithm.The volume fraction is φ ¼ rð4=3ÞpD3, where r = N/V is the numberdensity and V is the total volume. We define the reduced pressure p =PV/NkBT and the reduced stress s = SV/NkBT, where P and S are thepressure and the stress of the system, respectively. For simplicity, in therest of this paper, we refer as pressure and stress to p and s instead of Pand S. We set the Boltzmann constant kB, the temperature T, the meandiameter �D, and the particle mass m to unity.

Jin et al., Sci. Adv. 2018;4 : eaat6387 7 December 2018

Swap algorithmAt each dynamical step, the swap Monte Carlo algorithm attempts toexchange the positions of two randomly picked particles as long as theydo not overlap with their new neighbors. These nonlocal Monte Carlomoves eliminate the local confinement of particles in supercooled states,which, combined with standard event-driven MD, substantially facili-tates the equilibration procedure. It has been carefully examined that theswap algorithm does not introduce crystalline order in the polydisperseHS model studied here (20).

Compression/decompression algorithmWeused the Lubachevsky-Stillinger algorithm (58) to compress and de-compress the system. The particles were simulated by using event-driven MD. The sphere diameters were increased/decreased with a

constant rate. The MD time was expressed in units offfiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi1=kBm�D2

q.

Simple shear algorithmAt each step, we performedNcollision = 100 − 1000 collisions per particleusing the event-driven MD and then instantaneously increased theshear strain by dg ¼ :

gdt, where dt is the time elapsed during the colli-sions. The instantaneous shear shifts all particles by xi → xi + dgzi,where xi and zi are the x − and z −coordinates of particle i. To removethe possible overlappings introduced during this shift, we switched to aharmonic interparticle potential and used the conjugated gradient (CG)method to minimize the energy. The harmonic potential was switchedoff after CG. The Lees-Edwards boundary conditions (59) were used[see (24) for more details].

Protocols of ZFC and FCIn the ZFC protocol, starting from the initial equilibrium configurationat (D, g) = (0, 0), we (i) sheared the system to a target shear strain at (0, g)while keeping the volume strain unchanged, (ii) compressed it to a tar-get volume strain at (D, g) while keeping the shear strain unchanged, (iii)applied an additional small shear strain dg = 0.002, and (iv) measuredthe stresssZFC at the state point (D, g + dg). In the FCprotocol, the orderof steps (ii) and (iii) was interchanged. The FC protocol therefore hasthe path (0, 0) → (0, g)→ (0, g + dg)→ (D, g + dg). The target shearstrain was chosen such that it is below the yielding strain g < gY. Here,the shear strain serves as an external "field" with respect to compression,in analogy to the magnetic field in cooling experiments on spin glasses(43). The stress was measured on a time scale t = 10≈ 10t0, where t0 isthe ballistic time. This choice ensures that the ZFC protocol measuresthe short time response to shear, while the FC measurementcorresponds to the long time response because the shear strain g + dgwas reached before the volume strain was applied [see (24) for a detailedanalysis on the stress relaxation dynamics]. This protocol generalizesthe one used in (24), which corresponds to the case g = 0.

Protocols of CP-S, CV-S, and CS-C/DIn the CP-S protocol, the systemwas first compressed or decompressed(depending on whether the target p is higher or lower than pg) from theequilibrium state at (p, g) = (pg, 0) to the state at (p, 0). Then, simpleshear was applied under the constant-p condition, until the systemreached the target shear strain at (p, g). At each shear step, the particlediameters were adjusted to keep p constant. In the CV-S protocol, thesystem was first compressed or decompressed from φ = φg to the targetdensity φ, and then the simple shear was applied by keeping the volumeconstant. In the CS-C/D protocol, the system was first sheared from

10 of 12

SC I ENCE ADVANCES | R E S EARCH ART I C L E

http://advanceD

ownloaded from

(φ, g) = (φg, 0) to a target strain at (φg, g), and then compression ordecompression was applied while keeping the shear strain g constant.

Caging order parametersWeconsidered two order parametersDr andDAB defined below to char-acterize the glass state. The relative mean squared displacement isdefined as

Dr ¼ 1N∑N

i¼1ri � rri�� ��2 ð1Þ

where {ri} and frrig are the particle coordinates of the target andreference configurations. In Fig. 1, the target and reference are the con-figurations after and before shear, respectively. The replica meansquared displacement

DAB ¼ 1N∑N

i¼1rAi � r Bi�� ��2 ð2Þ

measures the distance between two replicas of the same sample gener-ated by two independent realizations.

One may also consider the time-dependent mean squared displace-ment DðtÞ ¼ 1

N ∑Ni¼1⟨jriðtÞ � rið0Þj2⟩, whose value at the ballistic time

scale t0 ~ 1 gives the typical vibrational cage size of particles. We foundthat in our systems, D(t0) ≲ 0.01 [see (23)]. The cage size is nearly un-changed under simple shear.

on March 29, 2020

s.sciencemag.org/

SUPPLEMENTARY MATERIALSSupplementary material for this article is available at http://advances.sciencemag.org/cgi/content/full/4/12/eaat6387/DC1Fig. S1. Singe-realization stress-strain curve for φg = 0.655 and D = 0.057.Fig. S2. Multicycle stress-strain curves.Fig. S3. Other representations of the stability-reversibility map.Fig. S4. Rescaled stress-strain curves.Fig. S5. Determination of the Gardner threshold for other φg.Fig. S6. Determination of the yielding-jamming crossover point.Fig. S7. Free-volume scalings in shear jamming.Fig. S8. Pressure susceptibility in the CS-C/D protocol.Fig. S9. Dependence of the stability-reversibility map on φg and protocols.Fig. S10. Dependence of the stability-reversibility map on the system size.Text S1. Bare and macro shear moduli.

REFERENCES AND NOTES1. W.-H. Wang, C. Dong, C. H. Shek, Bulk metallic glasses. Mater. Sci. Eng. R Rep. 44, 45–89

(2004).2. C. A. Angell, K. L. Ngai, G. B. McKenna, P. F. McMillan, S. W. Martin, Relaxation in

glassforming liquids and amorphous solids. J. Appl. Phys. 88, 3113–3157 (2000).3. A. Cavagna, Supercooled liquids for pedestrians. Phys. Rep. 476, 51–124 (2009).4. A. J. Liu, S. R. Nagel, The jamming transition and the marginally jammed solid. Annu. Rev.

Condens. Matter Phys. 1, 347–369 (2010).5. P. Charbonneau, J. Kurchan, G. Parisi, P. Urbani, F. Zamponi, Glass and jamming

transitions: From exact results to finite-dimensional descriptions. Annu. Rev. Condens.Matter Phys. 8, 265–288 (2017).

6. C. A. Schuh, T. C Hufnagel, U. Ramamurty, Mechanical behavior of amorphous alloys. ActaMater. 55, 4067–4109 (2007).

7. D. Rodney, A. Tanguy, D. Vandembroucq, Modeling the mechanics of amorphoussolids at different length scale and time scale. Model. Simul. Mat. Sci. Eng. 19, 083001(2011).

8. J.-L. Barrat, A. LemaÎtre, Heterogeneities in amorphous systems under shear, in DynamicalHeterogeneities in Glasses, Colloids, and Granular Media (OUP Oxford, 2011).

Jin et al., Sci. Adv. 2018;4 : eaat6387 7 December 2018

9. M. Ozawa, L. Berthier, G. Biroli, A. Rosso, G. Tarjus, A random critical point separatesbrittle and ductile yielding transitions in amorphous materials. arXiv:1803.11502[cond-mat.dis-nn] (30 March 2018).

10. D. Bonn, M. M. Denn, L. Berthier, T. Divoux, S. Manneville, Yield stress materials in softcondensed matter. Rev. Mod. Phys. 89, 035005 (2017).

11. M. Müller, M. Wyart, Marginal stability in structural, spin, and electron glasses. Annu. Rev.Condens. Matter Phys. 6, 177–200 (2015).

12. A. Nicolas, E. E. Ferrero, K. Martens, J.-L. Barrat, Deformation and flow of amorphoussolids: An updated review of mesoscale elastoplastic models. arXiv:1708.09194[cond-mat.dis-nn] (30 August 2017).

13. D. Bi, J. Zhang, B. Chakraborty, R. P. Behringer, Jamming by shear. Nature 480, 355–358(2011).

14. I. R. Peters, S. Majumdar, H. M. Jaeger, Direct observation of dynamic shear jamming indense suspensions. Nature 532, 214–217 (2016).

15. K. Hyun, M. Wilhelm, C. O. Klein, K. S. Cho, J. G. Nam, K. H. Ahn, S. J. Lee, R. H. Ewoldt,G. H. McKinley, A review of nonlinear oscillatory shear tests: Analysis and application oflarge amplitude oscillatory shear (LAOS). Prog. Polym. Sci. 36, 1697–1753 (2011).

16. I. Regev, J. Weber, C. Reichhardt, K. A. Dahmen, T. Lookman, Reversibility and criticality inamorphous solids. Nat. Commun. 6, 8805 (2015).

17. T. Kawasaki, L. Berthier, Macroscopic yielding in jammed solids is accompanied by anonequilibrium first-order transition in particle trajectories. Phys. Rev. E 94, 022615(2016).

18. P. Leishangthem, A. D. S. Parmar, S. Sastry, The yielding transition in amorphous solidsunder oscillatory shear deformation. Nat. Commun. 8, 14653 (2017).

19. W. G. T. Kranendonk, D. Frenkel, Computer simulation of solid-liquid coexistence in binaryhard sphere mixtures. Mol. Phys. 72, 679–697 (1991).

20. L. Berthier, D. Coslovich, A. Ninarello, M. Ozawa, Equilibrium sampling of hard spheres upto the jamming density and beyond. Phys. Rev. Lett. 116, 238002 (2016).

21. L. Berthier, P. Charbonneau, D. Coslovich, A. Ninarello, M. Ozawa, S. Yaida, Configurationalentropy measurements in extremely supercooled liquids that break the glass ceiling.Proc. Natl. Acad. Sci. U.S.A. 114, 11356–11361 (2017).

22. C. Rainone, P. Urbani, H. Yoshino, F. Zamponi, Following the evolution of hard sphereglasses in infinite dimensions under external perturbations: Compression and shearstrain. Phys. Rev. Lett. 114, 015701 (2015).

23. L. Berthier, P. Charbonneau, Y. Jin, G. Parisi, B. Seoane, F. Zamponi, Growing timescalesand lengthscales characterizing vibrations of amorphous solids. Proc. Natl. Acad. Sci. U.S.A.113, 8397–8401 (2016).

24. Y. Jin, H. Yoshino, Exploring the complex free-energy landscape of the simplest glass byrheology. Nat. Commun. 8, 14935 (2017).

25. A. J. Liu, S. R. Nagel, Jamming is not just cool anymore. Nature 396, 21–22 (1998).26. V. Trappe, V. Prasad, L. Cipelletti, P. N. Segre, D. A. Weitz, Jamming phase diagram for

attractive particles. Nature 411, 772–775 (2001).27. A. Ikeda, L. Berthier, P. Sollich, Unified study of glass and jamming rheology in soft

particle systems. Phys. Rev. Lett. 109, 018301 (2012).28. G. Biroli, P. Urbani, Liu-Nagel phase diagrams in infinite dimension. arXiv:1704.04649

[cond-mat.dis-nn] (15 April 2017).29. P. Urbani, F. Zamponi, Shear yielding and shear jamming of dense hard sphere glasses.

Phys. Rev. Lett. 118, 038001 (2017).30. R. Candelier, O. Dauchot, Creep motion of an intruder within a granular glass close to

jamming. Phys. Rev. Lett. 103, 128001 (2009).31. A. Seguin, O. Dauchot, Experimental evidence of the Gardner phase in a granular glass.

Phys. Rev. Lett. 117, 228001 (2016).32. M. L. Falk, J. S. Langer, Dynamics of viscoplastic deformation in amorphous solids.

Phys. Rev. E 57, 7192 (1998).33. H. G. E. Hentschel, S. Karmakar, E. Lerner, I. Procaccia, Do athermal amorphous solids

exist? Phys. Rev. E 83, 061101 (2011).34. J. Lin, T. Gueudré, A. Rosso, M. Wyart, Criticality in the approach to failure in amorphous

solids. Phys. Rev. Lett. 115, 168001 (2015).35. S. Franz, S. Spigler, Mean-field avalanches in jammed spheres. arXiv:1608.01265

[cond-mat.dis-nn] (3 August 2016).36. G. Biroli, P. Urbani, Breakdown of elasticity in amorphous solids. Nat. Phys. 12, 1130–1133

(2016).37. H. Yoshino, F. Zamponi, Shear modulus of glasses: Results from the full replica-symmetry-

breaking solution. Phys. Rev. E 90, 022302 (2014).38. C. Scalliet, L. Berthier, F. Zamponi, Absence of marginal stability in a structural glass.

Phys. Rev. Lett. 119, 205501 (2017).39. C. L. Hicks, M. J. Wheatley, M. J. Godfrey, M. A. Moore, Gardner transition in physical

dimensions. Phys. Rev. Lett. 120, 225501 (2018).

40. C. J. Fullerton, L. Berthier, Density controls the kinetic stability of ultrastable glasses.Europhys. Lett. 119, 36003 (2017).

41. S. Singh, M. D. Ediger, J. J. De Pablo, Ultrastable glasses from in silico vapour deposition.Nat. Mater. 12, 139–144 (2013).

11 of 12

SC I ENCE ADVANCES | R E S EARCH ART I C L E

httpD

ownloaded from

42. S. Karmakar, E. Lerner, I. Procaccia, J. Zylberg, Statistical physics of elastoplastic steadystates in amorphous solids: Finite temperatures and strain rates. Phys. Rev. E 82,031301 (2010).

43. S. Nagata, P. H. Keesom, H. R. Harrison, Low-dc-field susceptibility of Cu Mn spin glass.Phys. Rev. B 19, 1633–1638 (1979).

44. P.-E. Peyneau, J.-N. Roux, Frictionless bead packs have macroscopic friction, but nodilatancy. Phys. Rev. E 78, 011307 (2008).

45. J. C. Maxwell, L. On the calculation of the equilibrium and stiffness of frames. LED Philos.Mag. J. Sci. 27, 294–299 (1864).

46. M. Baity-Jesi, C. P. Goodrich, A. J Liu, S. R. Nagel, J. P Sethna, Emergent SO(3) symmetry ofthe frictionless shear jamming transition. J. Stat. Phys. 167, 735–748 (2017).

47. P. Urbani, G. Biroli, Gardner transition infinite dimensions. Phys. Rev. B 91, 100202 (2015).48. P. Charbonneau, S. Yaida, Nontrivial critical fixed point for replica-symmetry-breaking

transitions. Phys. Rev. Lett. 118, 215701 (2017).49. V. Lubchenko, P. G. Wolynes, Aging, jamming, and the limits of stability of amorphous

solids. J. Phys. Chem. B 122, 3280−3295 (2018).50. C. Rainone, P. Urbani, Following the evolution of glassy states under external perturbations:

The full replica symmetry breaking solution. J. Stat. Mech. Theor. Exp. 2016, 053302 (2016).

51. P. K. Jaiswal, I. Procaccia, C. Rainone, M. Singh, Mechanical yield in amorphous solids:A first-order phase transition. Phys. Rev. Lett. 116, 085501 (2016).

52. G. Parisi, I. Procaccia, C. Rainone, M. Singh, Shear bands as manifestation of a criticality inyielding amorphous solids. Proc. Natl. Acad. Sci. U.S.A. 114, 5577–5582 (2017).

53. A. Wisitsorasak, P. G. Wolynes, On the strength of glasses. Proc. Natl. Acad. Sci. U.S.A. 17,16068–16072 (2012).

54. M. L. Manning, A. J. Liu, Vibrational modes identify soft spots in a sheared disorderedpacking. Phys. Rev. Lett. 107, 108302 (2011).

55. H. Mizuno, H. Shiba, A. Ikeda, Continuum limit of the vibrational properties of amorphoussolids. Proc. Natl. Acad. Sci. U.S.A. 114, E9767–E9774 (2017).

56. E. Lerner, G. Düring, E. Bouchbinder, Statistics and properties of low-frequency vibrationalmodes in structural glasses. Phys. Rev. Lett. 117, 035501 (2016).

Jin et al., Sci. Adv. 2018;4 : eaat6387 7 December 2018

57. D. Fiocco, G. Foffi, S. Sastry, Oscillatory athermal quasistatic deformation of a model glass.Phys. Rev. E 88, 020301 (2013).

58. B. D. Lubachevsky, F. H. Stillinger, Geometric properties of random disk packings.J. Stat. Phys. 60, 561–583 (1990).

59. A. W. Lees, S. F. Edwards, The computer study of transport processes under extremeconditions. J. Phys. Condens. Matter 5, 1921 (1972).

Acknowledgments:We thank L. Berthier, M. Ozawa, C. Scalliet, M. Wyart, A. Altieri, O. Dauchot,K. Miyazaki, and T. Kawasaki for the discussions. Funding: This work was supported byKAKENHI (no. 25103005 “Fluctuation & Structure” and no. 50335337) from MEXT, Japan, by theCAS Pioneer Hundred Talents Program (Y.J.), by a grant from the Simons Foundation (no.454955, Francesco Zamponi), and by “Investissements d’Avenir” LabEx PALM (ANR-10-LABX-0039-PALM) (Pierfrancesco Urbani). The computations were performed using the computingfacilities in the Research Center for Computational Science, Okazaki, Japan, and in theCybermedia Center, Osaka University. Author contributions: Y.J., P.U., F.Z., and H.Y. designedthe research. Y.J. wrote the code and performed the numerical simulations and the dataanalysis, in close collaboration with H.Y. All authors contributed to the data analysis, thetheoretical interpretation of the results, and the writing of the manuscript. Competinginterests: The authors declare that they have no competing interests. Data and materialsavailability: All data needed to evaluate the conclusions in the paper are present in the paperand/or the Supplementary Materials. Additional data related to this paper may be requestedfrom the authors.

Submitted 20 March 2018Accepted 7 November 2018Published 7 December 201810.1126/sciadv.aat6387

Citation: Y. Jin, P. Urbani, F. Zamponi, H. Yoshino, A stability-reversibility map unifies elasticity,plasticity, yielding, and jamming in hard sphere glasses. Sci. Adv. 4, eaat6387 (2018).

://a

12 of 12

on March 29, 2020

dvances.sciencemag.org/

glassesA stability-reversibility map unifies elasticity, plasticity, yielding, and jamming in hard sphere

Yuliang Jin, Pierfrancesco Urbani, Francesco Zamponi and Hajime Yoshino

DOI: 10.1126/sciadv.aat6387 (12), eaat6387.4Sci Adv

ARTICLE TOOLS http://advances.sciencemag.org/content/4/12/eaat6387

MATERIALSSUPPLEMENTARY http://advances.sciencemag.org/content/suppl/2018/12/03/4.12.eaat6387.DC1

REFERENCES

http://advances.sciencemag.org/content/4/12/eaat6387#BIBLThis article cites 54 articles, 4 of which you can access for free

PERMISSIONS http://www.sciencemag.org/help/reprints-and-permissions

Terms of ServiceUse of this article is subject to the

is a registered trademark of AAAS.Science AdvancesYork Avenue NW, Washington, DC 20005. The title (ISSN 2375-2548) is published by the American Association for the Advancement of Science, 1200 NewScience Advances

License 4.0 (CC BY-NC).Science. No claim to original U.S. Government Works. Distributed under a Creative Commons Attribution NonCommercial Copyright © 2018 The Authors, some rights reserved; exclusive licensee American Association for the Advancement of

on March 29, 2020

http://advances.sciencemag.org/

Dow

nloaded from

Recommended